Development of Simulation Tools for Selective Laser Melting Additive
Thomas Nolan*, Yongsheng Lian*, Mark Sussman†
*Department of Mechanical Engineering, University of Louisville, Louisville, KY
†Department of Mathematics, Florida State University, Tallahassee, FL
Two simulations tools have been developed to simulate selective laser melting. One is based on a
multiphase flow solver with dynamic mesh adaptation and massive parallelism. The simulation
tool is based on a first-principles approach to simulate complex additive manufacturing processes
at the entire built part/component level. The developed model takes into account of heating,
melting, powder-to-solid volumetric consolidation, cooling, as well as solidification and shrinkage
that are often ignored in current simulation tools. The second tool is to solve the heat equation only
without considering the flow field and volumetric changes. In both tools laser is modeled as a heat
source. The reported work is our first step toward the development of a complete software suite
that can be executed rapidly on workstations and clusters with accelerators. The simulation tool
can provide AM practitioners and researchers from industry and academic a fast and accurate
simulation-based approach to replace current trial-and-error based practices in industry for process
and material development.
Laser and metal powder based additive manufacturing (AM), specifically Laser sintering (LS) and
Direct Digital Manufacturing (DDM), offers design freedom over the constraints of traditional
manufacturing methods [1, 2]. LS is a process in which a high-energy laser beam scans a powder
bed surface to melt the powder (ceramics, metal, or polymer) to form a bulk part . The most
common terminology for LS of metals is Selective Laser Melting (SLM) . SLM can benefit
from better design and lower cost, but LS is complicated due to the fast laser scanning rates and
complex heat transfer and phase change processes [5-7]. There is a poor understanding of the
important physical processes dealing with laser-material interactions, the heat transfer and molten
metal flow, and metal phase transformations and thermal stresses, which hinders quality of a
finished bulk part, such as density, dimensions, mechanical properties, and microstructure [7, 8].
Previous research also found the temperature field was inhomogeneous [9-13]. And large thermal
gradients increase residual stresses and deformation in metals and may lead to crack formation in
a bulk part, which leads to the develop of serious problem in the SLM process .
Due to the importance of temperature distribution in LS, researchers have grown towards
understanding the SLM process [10, 15-19] and creating models to describe the thermal evolution
of LS [5, 9, 11, 20-22]. Simulation models can demonstrate the influence of various parameters
and are essential tools for identifying the proper parameters without expensive experimental
Various heat transfer processes occur in the SLM. Figure 1 shows the representation of heat
transfer in SLM . It consists of radiation at the powder bed, convection between the powder
bed and the environment of an air void or gas filled chamber, and heat conduction inside the
powder bed and between the bed and substrate. The powder phase change is another important
phenomenon in SLM, and phase change can significantly change thermal properties of the powder
Figure 1. Schematic representation of heat transfer
SLM metal temperature distribution has been modeled with heat equations without considering
the flow field [13, 23-29]. Some researchers ignore the heat source as internal energy [30-32], but
other studies put the source into the boundary condition equation [5, 20]. Other employ phase
change and enthalpy to study the temperature field in SLM [5, 20, 30]. Another model considers
influence from metal powder shrinkage and the molten pool fluid flow. Chan and Mazumder
showed that fluid flow through the molten pool had a significant effect of the homogeneity of the
sintering weld . Some consider that the molten pool influences the thermal field in SLM. The
model to simulate melting and solidification has been developed and used by [34-40]. One-
dimensional melting in mixed powders has been solved analytically by . A three-dimensional
model has been created that considers the thermal behavior and fluid dynamics in the molten pool
caused by Marangoni and buoyancy forces along with the melt pool flow caused by gravity and
capillary forces . The model also accounts for powder shrinkage due to density and uses a
fixed grid temperature transfer model for modeling the melting and solidification of the powder.
The model has been compared to the cross-sectional profile for the melt-solid interface in laser
processing for nonporous metal experiments. The results show that the thermocapillary force,
shrinkage, and buoyancy force dominate the melting and fluid flow .
Another thermal evolution of SLM as a heat transfer process utilizes the Fourier heat conduction
theory with a Gaussian laser source embedded as an internal energy and the volume-of-fluid
method to study the multiphase interaction forces and temperature variation in Ti-6Al-4V powder.
Unlike the model from , the Marangoni and buoyancy forces are not considered. The latent
heat is dependent on temperature and considers liquid phase of the powder particles. The model
uses a volume fraction transport equation to present the distribution of metal and gas phase within
the computation domain. The model has been compared to a cross-sectional profile for the
distribution of the melting pool.
Various models have been proposed to model the heat transfer from laser beam. Some models
have sought to use the volumetric laser beam distribution assumption. Niebling and Otto
considered a volumetric line heat source . Gusarov and Yadroitsev used a radiation transfer
equation with an isotropic scattering term to describe laser beam penetration . Although the
laser beam penetration problem has been studied, Kolossov and Boillat found that with an element
size larger than five gradient diameters, the laser beam penetration can be ignored . Realizing
the interaction between the laser beam and powder bed, leads to a greater understanding of laser
beam penetration and absorption. Several models consider the absorption a constant ratio for the
bulk powder [20, 45, 47-50]. Laser beam absorption in powder depends on several factors
including oxidation level, surface type, surface temperature, and laser beam wavelength. In the
case of metal powders, the laser beam absorption ratio varies within a few percent of the molten
absorption ratio .
Thermal properties of metal powder include density, enthalpy, heat capacity, and thermal
conductivity. Carslaw and Jaeger show that thermal conductivity varies with temperature .
SLM uses an effective thermal conductivity. It has also been shown that the porosity of the powder
bed influences thermal conductivity. The effective thermal conductivity is a function of the thermal
conductivities of solid metal and gas in the powder voids [3, 20, 51].
The main consideration of thermal conductivity of metal powders is the temperature near the
melting point and above in liquid state. Without experimental data, a constant thermal conductivity
is assumed. Thummler proposed that thermal conductivity is influenced by powder porosity and
pore geometries and thermal conductivity is controlled by gas content in the voids of the powder
. Rombouts et al. showed that thermal conductivity is independent of powder material and
depends on porosity and size of voids in the powder along with depending on gas content in the
voids . Roberts and Wang show that the thermal conductivity of Ti6Al4V powder is low for
powder and increases dramatically when nearing the melting point . The density and heat
capacity of metal powder is shown as the mass average of each state’s (powder, liquid, solid) value
. Some consider the heat capacity to be separate at each phase and use an effective heat
capacity that is temperature dependent .
In this paper, we present two models to study SLM. One is based on commercial software Fluent,
and the other one is based on an in house multiphase flow solver. In the first approach, we solve
the heat transfer equations without considering the flow field. The laser is modeled as a three-
dimensional Gaussian energy source that is imposed on a two-dimensional surface. This approach
only considers the heat transfer without the phase change. In the second approach, we will model
the phase change using multiphase flow solver.
In the following we introduce the two models used to study SLM. The first one is based on a simple
heat equation (the heat conduction model